#------------------------------------------------------------------------------
#$Date: 2021-04-12 11:27:20 +0300 (Mon, 12 Apr 2021) $
#$Revision: 264049 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/16/1561652.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561652
loop_
_publ_author_name
'Baranets, Sviatoslav'
'Darone, Gregory M.'
'Bobev, Svilen'
_publ_section_title
;
 Synthesis and structure of Sr14Zn1+As11 and Eu14Zn1+As11 (x ≤
 0.5). New members of the family of pnictides isotypic with Ca14AlSb11,
 exhibiting a new type of structural disorder
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              120990
_journal_paper_doi               10.1016/j.jssc.2019.120990
_journal_volume                  280
_journal_year                    2019
_chemical_formula_sum            'As11 Sr14 Zn1.33'
_chemical_formula_weight         2137.99
_space_group_crystal_system      tetragonal
_space_group_IT_number           142
_space_group_name_Hall           '-I 4bd 2c'
_space_group_name_H-M_alt        'I 41/a c d :2'
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_audit_contact_author_name
;
;
_audit_creation_date             2019-08-13
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   16.5172(19)
_cell_length_b                   16.5172(19)
_cell_length_c                   22.193(3)
_cell_measurement_reflns_used    2685
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      24.85
_cell_measurement_theta_min      3.49
_cell_volume                     6054.6(13)
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      200.0
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1026
_diffrn_reflns_av_unetI/netI     0.0437
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       30
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_number            37775
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.814
_diffrn_reflns_theta_min         2.466
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    37.397
_exptl_absorpt_correction_T_max  0.0497
_exptl_absorpt_correction_T_min  0.0136
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1634 before and 0.0562 after correction. The Ratio of minimum to maximum transmission is 0.2736. The λ/2 correction factor is Not present.'
_exptl_crystal_colour            grey
_exptl_crystal_density_diffrn    4.691
_exptl_crystal_description       irregular
_exptl_crystal_F_000             7480
_exptl_crystal_size_max          0.141
_exptl_crystal_size_mid          0.136
_exptl_crystal_size_min          0.108
_refine_diff_density_max         1.756
_refine_diff_density_min         -1.745
_refine_diff_density_rms         0.291
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.066
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     80
_refine_ls_number_reflns         2176
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.066
_refine_ls_R_factor_all          0.0696
_refine_ls_R_factor_gt           0.0436
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0374P)²+192.1502P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0978
_refine_ls_wR_factor_ref         0.1105
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                1610
_reflns_number_total             2176
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            JSSC-2019-120990.cif
_cod_data_source_block           II
_cod_original_cell_volume        6054.7(16)
_cod_original_sg_symbol_H-M      'I 41/a c d'
_cod_database_code               1561652
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.107
_shelx_estimated_absorpt_t_min   0.077
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(Sr4A) = Uanis(Sr4B)
Uanis(Sr2A) = Uanis(Sr2B)
2. Others
 Sof(Sr2B)=Sof(Sr4B)=1-FVAR(1)
 Sof(Sr2A)=Sof(Sr4A)=FVAR(1)
 Fixed Sof: As4(0.25)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-y+1/4, x+3/4, z+1/4'
'y+1/4, -x+1/4, z+3/4'
'-x+1/2, y, -z'
'x, -y, -z+1/2'
'y+1/4, x+3/4, -z+3/4'
'-y+1/4, -x+1/4, -z+1/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-y+3/4, x+5/4, z+3/4'
'y+3/4, -x+3/4, z+5/4'
'-x+1, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1'
'y+3/4, x+5/4, -z+5/4'
'-y+3/4, -x+3/4, -z+3/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'y-1/4, -x-3/4, -z-1/4'
'-y-1/4, x-1/4, -z-3/4'
'x-1/2, -y, z'
'-x, y, z-1/2'
'-y-1/4, -x-3/4, z-3/4'
'y-1/4, x-1/4, z-1/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'y+1/4, -x-1/4, -z+1/4'
'-y+1/4, x+1/4, -z-1/4'
'x, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
'-y+1/4, -x-1/4, z-1/4'
'y+1/4, x+1/4, z+1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Sr1 Sr 0.04463(5) 0.07165(5) 0.17166(4) 0.0266(2) Uani 1 1 d . . . . .
Sr2A Sr 0.02347(10) 0.37537(11) 0.00252(7) 0.0271(3) Uani 0.8458(19) 1 d . . .
. .
Sr2B Sr 0.0126(7) 0.3661(7) 0.0157(5) 0.0271(3) Uani 0.1542(19) 1 d . . . . .
Sr3 Sr 0.35394(8) 0.000000 0.250000 0.0315(3) Uani 1 2 d S T P . .
Sr4A Sr 0.34891(6) 0.07150(6) 0.09509(4) 0.0251(2) Uani 0.8458(19) 1 d . . . .
.
Sr4B Sr 0.3152(3) 0.0350(3) 0.0686(2) 0.0251(2) Uani 0.1542(19) 1 d . . . . .
Zn1 Zn 0.000000 0.250000 0.375000 0.0257(4) Uani 1 4 d S T P . .
Zn2 Zn 0.3615(8) 0.1577(8) 0.1421(5) 0.031(4) Uani 0.084(5) 1 d . . . . .
As1 As 0.13253(6) 0.38253(6) 0.125000 0.0267(3) Uani 1 2 d S T P . .
As2 As 0.36532(5) 0.25269(6) 0.05934(4) 0.0239(2) Uani 1 1 d . . . . .
As3 As 0.13019(7) 0.02391(6) 0.04667(4) 0.0319(2) Uani 1 1 d . . . . .
As4 As 0.01498(9) 0.26498(9) 0.125000 0.0238(6) Uani 0.5 2 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Sr2B Sr1 Sr2B 101.4(3) 15_444 10_454
Sr4A Sr1 Sr2B 121.2(2) 8 15_444
Sr4A Sr1 Sr2B 105.98(19) 8 10_454
Sr4A Sr1 Sr4B 16.08(9) 8 8
Sr4B Sr1 Sr2B 105.4(2) 8 15_444
Sr4B Sr1 Sr2B 115.1(2) 8 10_454
Zn2 Sr1 Sr2B 85.3(3) 8 10_454
Zn2 Sr1 Sr2B 147.8(3) 8 15_444
Zn2 Sr1 Sr4A 29.2(2) 8 8
Zn2 Sr1 Sr4B 45.2(2) 8 8
As1 Sr1 Sr2B 53.3(2) 10_454 10_454
As1 Sr1 Sr2B 102.4(2) 10_454 15_444
As1 Sr1 Sr4A 135.59(3) 10_454 8
As1 Sr1 Sr4B 151.67(10) 10_454 8
As1 Sr1 Zn2 106.6(2) 10_454 8
As1 Sr1 As2 92.72(3) 10_454 8
As1 Sr1 As2 91.84(3) 10_454 3_545
As1 Sr1 As3 100.44(3) 10_454 .
As1 Sr1 As4 62.99(4) 10_454 .
As2 Sr1 Sr2B 61.6(2) 3_545 15_444
As2 Sr1 Sr2B 138.9(2) 3_545 10_454
As2 Sr1 Sr2B 108.96(17) 8 10_454
As2 Sr1 Sr2B 149.39(19) 8 15_444
As2 Sr1 Sr4A 114.86(3) 3_545 8
As2 Sr1 Sr4A 53.91(3) 8 8
As2 Sr1 Sr4B 105.72(9) 3_545 8
As2 Sr1 Sr4B 65.21(9) 8 8
As2 Sr1 Zn2 42.5(2) 8 8
As2 Sr1 Zn2 129.9(2) 3_545 8
As2 Sr1 As2 91.81(3) 8 3_545
As2 Sr1 As4 155.44(5) 8 .
As2 Sr1 As4 92.50(3) 3_545 .
As3 Sr1 Sr2B 51.5(2) . 10_454
As3 Sr1 Sr2B 113.6(2) . 15_444
As3 Sr1 Sr2B 112.00(19) 8 10_454
As3 Sr1 Sr2B 52.7(2) 8 15_444
As3 Sr1 Sr4A 56.53(3) . 8
As3 Sr1 Sr4A 68.88(3) 8 8
As3 Sr1 Sr4B 63.62(8) . 8
As3 Sr1 Sr4B 53.82(10) 8 8
As3 Sr1 Zn2 95.5(2) 8 8
As3 Sr1 Zn2 47.6(2) . 8
As3 Sr1 As1 151.13(4) 8 10_454
As3 Sr1 As2 89.11(3) . 8
As3 Sr1 As2 116.15(4) 8 8
As3 Sr1 As2 167.63(4) . 3_545
As3 Sr1 As2 87.89(3) 8 3_545
As3 Sr1 As3 80.65(4) 8 .
As3 Sr1 As4 88.17(4) 8 .
As3 Sr1 As4 91.77(3) . .
As4 Sr1 Sr2B 54.62(18) . 10_454
As4 Sr1 Sr2B 50.23(18) 10_454 10_454
As4 Sr1 Sr2B 49.34(19) . 15_444
As4 Sr1 Sr2B 57.9(2) 10_454 15_444
As4 Sr1 Sr4A 148.70(4) 10_454 8
As4 Sr1 Sr4A 142.52(4) . 8
As4 Sr1 Sr4B 135.97(9) . 8
As4 Sr1 Sr4B 145.45(9) 10_454 8
As4 Sr1 Zn2 137.5(2) . 8
As4 Sr1 Zn2 135.5(2) 10_454 8
As4 Sr1 As1 52.08(5) 10_454 10_454
As4 Sr1 As2 144.63(5) 10_454 8
As4 Sr1 As2 92.60(3) 10_454 3_545
As4 Sr1 As3 99.08(5) 10_454 8
As4 Sr1 As3 93.78(3) 10_454 .
As4 Sr1 As4 10.91(7) 10_454 .
Sr3 Sr2A Sr1 150.93(5) 27_565 15_444
Sr4A Sr2A Sr1 70.98(4) 14_454 15_444
Sr4A Sr2A Sr3 138.02(4) 14_454 27_565
Zn1 Sr2A Sr1 92.90(4) 29_554 15_444
Zn1 Sr2A Sr3 98.68(4) 29_554 27_565
Zn1 Sr2A Sr4A 65.50(3) 29_554 14_454
Zn1 Sr2A As2 43.59(3) 29_554 14_454
Zn1 Sr2A As4 101.93(5) 29_554 10_454
Zn2 Sr2A Sr1 139.8(3) 31_565 15_444
Zn2 Sr2A Sr3 64.0(3) 31_565 27_565
Zn2 Sr2A Sr4A 77.3(3) 31_565 14_454
Zn2 Sr2A Zn1 50.8(3) 31_565 29_554
Zn2 Sr2A As1 121.2(3) 31_565 .
Zn2 Sr2A As2 52.8(3) 31_565 5
Zn2 Sr2A As2 90.4(3) 31_565 14_454
Zn2 Sr2A As3 124.8(3) 31_565 10_454
Zn2 Sr2A As3 53.2(3) 31_565 26
Zn2 Sr2A As4 143.3(3) 31_565 10_454
Zn2 Sr2A As4 144.3(3) 31_565 .
As1 Sr2A Sr1 97.05(4) . 15_444
As1 Sr2A Sr3 57.27(3) . 27_565
As1 Sr2A Sr4A 155.02(6) . 14_454
As1 Sr2A Zn1 138.60(6) . 29_554
As1 Sr2A As2 137.16(5) . 14_454
As1 Sr2A As4 59.72(4) . 10_454
As1 Sr2A As4 49.66(5) . .
As2 Sr2A Sr1 118.18(5) 5 15_444
As2 Sr2A Sr1 50.18(3) 14_454 15_444
As2 Sr2A Sr3 57.03(4) 5 27_565
As2 Sr2A Sr3 139.80(5) 14_454 27_565
As2 Sr2A Sr4A 50.07(3) 14_454 14_454
As2 Sr2A Sr4A 111.16(5) 5 14_454
As2 Sr2A Zn1 46.96(3) 5 29_554
As2 Sr2A As1 93.80(5) 5 .
As2 Sr2A As2 82.91(5) 5 14_454
As2 Sr2A As3 91.37(4) 5 26
As2 Sr2A As3 163.95(7) 5 10_454
As2 Sr2A As4 91.04(5) 5 10_454
As2 Sr2A As4 91.68(5) 5 .
As3 Sr2A Sr1 51.39(3) 10_454 15_444
As3 Sr2A Sr1 149.59(6) 26 15_444
As3 Sr2A Sr3 51.62(3) 26 27_565
As3 Sr2A Sr3 138.56(6) 10_454 27_565
As3 Sr2A Sr4A 92.71(4) 26 14_454
As3 Sr2A Sr4A 55.79(4) 10_454 14_454
As3 Sr2A Zn1 103.65(4) 26 29_554
As3 Sr2A Zn1 117.73(6) 10_454 29_554
As3 Sr2A As1 99.47(5) 10_454 .
As3 Sr2A As1 87.28(5) 26 .
As3 Sr2A As2 81.23(4) 10_454 14_454
As3 Sr2A As2 135.34(5) 26 14_454
As3 Sr2A As3 98.20(5) 10_454 26
As3 Sr2A As4 136.93(7) 26 .
As3 Sr2A As4 146.99(7) 26 10_454
As3 Sr2A As4 87.92(3) 10_454 10_454
As3 Sr2A As4 90.07(4) 10_454 .
As4 Sr2A Sr1 47.16(3) 10_454 15_444
As4 Sr2A Sr1 54.88(3) . 15_444
As4 Sr2A Sr3 104.09(5) 10_454 27_565
As4 Sr2A Sr3 96.06(5) . 27_565
As4 Sr2A Sr4A 116.89(5) 10_454 14_454
As4 Sr2A Sr4A 125.63(5) . 14_454
As4 Sr2A Zn1 109.52(5) . 29_554
As4 Sr2A As2 77.59(4) 10_454 14_454
As4 Sr2A As2 87.63(5) . 14_454
As4 Sr2A As4 10.06(6) . 10_454
Sr1 Sr2B Sr1 61.07(15) 15_444 10_454
Sr1 Sr2B Sr4A 110.2(3) 10_454 14_454
Sr1 Sr2B Sr4A 73.7(2) 15_444 14_454
Sr1 Sr2B Zn1 96.1(3) 15_444 29_554
Zn1 Sr2B Sr1 156.7(3) 29_554 10_454
Zn1 Sr2B Sr4A 63.3(2) 29_554 14_454
Zn2 Sr2B Sr1 154.9(5) 31_565 10_454
Zn2 Sr2B Sr1 138.8(5) 31_565 15_444
Zn2 Sr2B Sr4A 72.2(3) 31_565 14_454
Zn2 Sr2B Zn1 47.6(3) 31_565 29_554
Zn2 Sr2B As1 114.2(4) 31_565 .
Zn2 Sr2B As2 48.5(3) 31_565 5
Zn2 Sr2B As2 86.6(4) 31_565 14_454
Zn2 Sr2B As3 47.5(3) 31_565 26
Zn2 Sr2B As4 143.2(5) 31_565 10_454
As1 Sr2B Sr1 54.56(18) . 10_454
As1 Sr2B Sr1 106.2(3) . 15_444
As1 Sr2B Sr4A 157.6(4) . 14_454
As1 Sr2B Zn1 137.5(4) . 29_554
As1 Sr2B As2 93.1(3) . 5
As1 Sr2B As2 147.5(3) . 14_454
As1 Sr2B As3 83.8(3) . 26
As1 Sr2B As4 64.8(2) . 10_454
As2 Sr2B Sr1 143.1(4) 5 10_454
As2 Sr2B Sr1 123.5(4) 5 15_444
As2 Sr2B Sr1 53.51(17) 14_454 15_444
As2 Sr2B Sr1 114.5(3) 14_454 10_454
As2 Sr2B Sr4A 105.6(3) 5 14_454
As2 Sr2B Sr4A 49.97(17) 14_454 14_454
As2 Sr2B Zn1 43.24(15) 14_454 29_554
As2 Sr2B Zn1 44.84(16) 5 29_554
As2 Sr2B As2 82.2(3) 5 14_454
As2 Sr2B As3 83.2(2) 5 26
As2 Sr2B As4 94.9(3) 5 10_454
As3 Sr2B Sr1 55.85(18) 10_454 15_444
As3 Sr2B Sr1 149.8(4) 26 15_444
As3 Sr2B Sr1 55.39(18) 10_454 10_454
As3 Sr2B Sr1 107.4(3) 26 10_454
As3 Sr2B Sr4A 86.4(2) 26 14_454
As3 Sr2B Sr4A 55.6(2) 10_454 14_454
As3 Sr2B Zn1 117.3(4) 10_454 29_554
As3 Sr2B Zn1 94.8(2) 26 29_554
As3 Sr2B Zn2 117.5(5) 10_454 31_565
As3 Sr2B As1 105.1(4) 10_454 .
As3 Sr2B As2 127.0(3) 26 14_454
As3 Sr2B As2 161.2(4) 10_454 5
As3 Sr2B As2 84.6(3) 10_454 14_454
As3 Sr2B As3 94.2(3) 10_454 26
As3 Sr2B As4 96.8(3) 10_454 10_454
As4 Sr2B Sr1 52.83(17) . 10_454
As4 Sr2B Sr1 57.41(16) 10_454 10_454
As4 Sr2B Sr1 60.90(17) . 15_444
As4 Sr2B Sr1 52.00(14) 10_454 15_444
As4 Sr2B Sr4A 134.2(3) . 14_454
As4 Sr2B Sr4A 124.0(3) 10_454 14_454
As4 Sr2B Zn1 106.0(3) 10_454 29_554
As4 Sr2B Zn1 113.9(4) . 29_554
As4 Sr2B Zn2 143.1(5) . 31_565
As4 Sr2B As1 53.5(2) . .
As4 Sr2B As2 94.7(3) . 14_454
As4 Sr2B As2 83.5(2) 10_454 14_454
As4 Sr2B As2 95.0(3) . 5
As4 Sr2B As3 99.3(3) . 10_454
As4 Sr2B As3 148.4(4) 10_454 26
As4 Sr2B As3 137.2(4) . 26
As4 Sr2B As4 11.31(8) . 10_454
Sr4A Sr3 Sr4A 177.38(5) 6 .
Sr4B Sr3 Sr4A 110.54(10) 8 6
Sr4B Sr3 Sr4A 67.28(10) 3_545 6
Sr4B Sr3 Sr4A 110.54(10) 3_545 .
Sr4B Sr3 Sr4A 67.28(10) 8 .
Sr4B Sr3 Sr4B 78.2(2) 8 3_545
Sr4B Sr3 Zn2 87.0(2) 8 .
Sr4B Sr3 Zn2 96.2(2) 3_545 .
Sr4B Sr3 Zn2 87.0(2) 3_545 6
Sr4B Sr3 Zn2 96.2(2) 8 6
Sr4B Sr3 As1 54.67(10) 8 20_656
Sr4B Sr3 As1 54.67(10) 3_545 25
Sr4B Sr3 As1 132.88(11) 8 25
Sr4B Sr3 As1 132.88(11) 3_545 20_656
Sr4B Sr3 As2 124.02(10) 8 20_656
Sr4B Sr3 As2 124.02(10) 3_545 23_666
Sr4B Sr3 As2 123.37(11) 3_545 20_656
Sr4B Sr3 As2 123.37(11) 8 23_666
Sr4B Sr3 As3 61.83(11) 3_545 3_545
Sr4B Sr3 As3 53.55(10) 8 3_545
Sr4B Sr3 As3 53.55(10) 3_545 8
Sr4B Sr3 As3 61.83(11) 8 8
Zn2 Sr3 Sr4A 28.6(2) . .
Zn2 Sr3 Sr4A 151.6(2) . 6
Zn2 Sr3 Sr4A 151.6(2) 6 .
Zn2 Sr3 Sr4A 28.6(2) 6 6
Zn2 Sr3 Zn2 175.9(4) 6 .
As1 Sr3 Sr4A 54.13(2) 20_656 .
As1 Sr3 Sr4A 54.14(2) 25 6
As1 Sr3 Sr4A 126.08(2) 25 .
As1 Sr3 Sr4A 126.08(2) 20_656 6
As1 Sr3 Zn2 82.3(2) 20_656 .
As1 Sr3 Zn2 82.3(2) 25 6
As1 Sr3 Zn2 97.5(2) 20_656 6
As1 Sr3 Zn2 97.5(2) 25 .
As1 Sr3 As1 172.45(5) 25 20_656
As2 Sr3 Sr4A 56.88(2) 23_666 6
As2 Sr3 Sr4A 125.39(4) 23_666 .
As2 Sr3 Sr4A 125.39(4) 20_656 6
As2 Sr3 Sr4A 56.88(2) 20_656 .
As2 Sr3 Zn2 131.8(2) 20_656 6
As2 Sr3 Zn2 44.2(2) 23_666 6
As2 Sr3 Zn2 131.8(2) 23_666 .
As2 Sr3 Zn2 44.2(2) 20_656 .
As2 Sr3 As1 87.09(3) 23_666 20_656
As2 Sr3 As1 87.52(2) 23_666 25
As2 Sr3 As1 87.09(3) 20_656 25
As2 Sr3 As1 87.52(2) 20_656 20_656
As2 Sr3 As2 88.72(4) 20_656 23_666
As3 Sr3 Sr4A 120.80(4) 8 6
As3 Sr3 Sr4A 57.08(2) 3_545 6
As3 Sr3 Sr4A 57.08(2) 8 .
As3 Sr3 Sr4A 120.80(4) 3_545 .
As3 Sr3 Zn2 47.4(2) 8 .
As3 Sr3 Zn2 136.6(2) 8 6
As3 Sr3 Zn2 136.6(2) 3_545 .
As3 Sr3 Zn2 47.4(2) 3_545 6
As3 Sr3 As1 97.93(3) 8 20_656
As3 Sr3 As1 97.93(3) 3_545 25
As3 Sr3 As1 87.28(2) 8 25
As3 Sr3 As1 87.28(2) 3_545 20_656
As3 Sr3 As2 89.25(2) 8 20_656
As3 Sr3 As2 174.51(3) 8 23_666
As3 Sr3 As2 89.25(2) 3_545 23_666
As3 Sr3 As2 174.51(3) 3_545 20_656
As3 Sr3 As3 93.22(5) 3_545 8
Sr1 Sr4A Sr2A 113.72(3) 8 14_554
Sr1 Sr4A Sr2B 108.87(16) 8 14_554
Sr1 Sr4A Sr3 108.36(3) 8 .
Sr1 Sr4A Sr4B 87.74(8) 8 8
Sr2A Sr4A Sr2B 5.59(14) 14_554 14_554
Sr3 Sr4A Sr2A 127.65(4) . 14_554
Sr3 Sr4A Sr2B 133.17(14) . 14_554
Sr3 Sr4A Sr4B 47.56(8) . 8
Sr4B Sr4A Sr1 82.8(3) . 8
Sr4B Sr4A Sr2A 155.75(9) 8 14_554
Sr4B Sr4A Sr2A 103.3(3) . 14_554
Sr4B Sr4A Sr2B 158.1(2) 8 14_554
Sr4B Sr4A Sr2B 100.2(3) . 14_554
Sr4B Sr4A Sr3 111.7(3) . .
Sr4B Sr4A Sr4B 66.8(3) . 8
Sr4B Sr4A Zn2 152.3(5) . .
Sr4B Sr4A As1 65.9(3) . 20_656
Sr4B Sr4A As2 155.4(3) . 20_656
Sr4B Sr4A As2 118.3(3) . .
Sr4B Sr4A As3 49.7(3) . 5
Sr4B Sr4A As3 103.5(3) . 8
Zn2 Sr4A Sr1 70.2(4) . 8
Zn2 Sr4A Sr2A 93.6(4) . 14_554
Zn2 Sr4A Sr2B 94.5(5) . 14_554
Zn2 Sr4A Sr3 72.7(4) . .
Zn2 Sr4A Sr4B 104.8(4) . 8
Zn2 Sr4A As1 130.3(4) . 20_656
Zn2 Sr4A As2 50.5(4) . 20_656
Zn2 Sr4A As2 50.8(4) . .
Zn2 Sr4A As3 56.1(4) . 8
Zn2 Sr4A As3 138.3(4) . 5
As1 Sr4A Sr1 133.96(4) 20_656 8
As1 Sr4A Sr2A 106.07(4) 20_656 14_554
As1 Sr4A Sr2B 109.30(18) 20_656 14_554
As1 Sr4A Sr3 59.055(16) 20_656 .
As1 Sr4A Sr4B 49.83(9) 20_656 8
As1 Sr4A As2 90.54(3) 20_656 20_656
As1 Sr4A As3 98.39(3) 20_656 8
As1 Sr4A As3 87.42(3) 20_656 5
As2 Sr4A Sr1 120.64(3) 20_656 8
As2 Sr4A Sr1 56.67(3) . 8
As2 Sr4A Sr2A 63.62(4) . 14_554
As2 Sr4A Sr2A 75.40(3) 20_656 14_554
As2 Sr4A Sr2B 60.73(18) . 14_554
As2 Sr4A Sr2B 80.14(16) 20_656 14_554
As2 Sr4A Sr3 123.51(3) . .
As2 Sr4A Sr3 56.64(3) 20_656 .
As2 Sr4A Sr4B 104.11(9) 20_656 8
As2 Sr4A Sr4B 140.61(9) . 8
As2 Sr4A As1 169.14(4) . 20_656
As2 Sr4A As2 83.62(4) . 20_656
As2 Sr4A As3 90.38(3) . 8
As2 Sr4A As3 88.66(3) . 5
As3 Sr4A Sr1 55.67(3) 8 8
As3 Sr4A Sr1 97.54(3) 5 8
As3 Sr4A Sr2A 149.30(5) 8 14_554
As3 Sr4A Sr2A 53.96(3) 5 14_554
As3 Sr4A Sr2B 149.09(19) 8 14_554
As3 Sr4A Sr2B 50.61(18) 5 14_554
As3 Sr4A Sr3 146.25(3) 5 .
As3 Sr4A Sr3 52.70(3) 8 .
As3 Sr4A Sr4B 52.58(9) 8 8
As3 Sr4A Sr4B 114.58(10) 5 8
As3 Sr4A As2 86.27(3) 8 20_656
As3 Sr4A As2 126.19(4) 5 20_656
As3 Sr4A As3 147.13(5) 8 5
Sr1 Sr4B Sr4A 93.03(12) 8 8
Sr1 Sr4B Sr4B 71.80(13) 8 5
Sr1 Sr4B As2 52.12(7) 8 .
Sr3 Sr4B Sr1 114.01(17) 4_554 8
Sr3 Sr4B Sr4A 65.16(11) 4_554 8
Sr3 Sr4B Sr4B 50.90(10) 4_554 5
Sr3 Sr4B Sr4B 79.9(2) 4_554 8
Sr3 Sr4B As2 143.90(17) 4_554 .
Sr3 Sr4B As3 125.33(17) 4_554 8
Sr3 Sr4B As3 60.94(11) 4_554 .
Sr4A Sr4B Sr1 81.1(3) . 8
Sr4A Sr4B Sr3 164.6(4) . 4_554
Sr4A Sr4B Sr4A 113.1(3) . 8
Sr4A Sr4B Sr4B 97.4(4) . 8
Sr4A Sr4B Sr4B 94.02(17) 8 5
Sr4A Sr4B Sr4B 142.5(3) . 5
Sr4A Sr4B Zn2 17.8(4) . .
Sr4A Sr4B As1 95.9(3) . 20_656
Sr4A Sr4B As2 47.7(2) . .
Sr4A Sr4B As3 113.9(4) . 5
Sr4A Sr4B As3 132.1(4) . .
Sr4A Sr4B As3 60.7(3) . 8
Sr4B Sr4B Sr1 91.74(8) 8 8
Sr4B Sr4B Sr4A 15.71(11) 8 8
Sr4B Sr4B Sr4B 108.5(2) 8 5
Sr4B Sr4B As2 128.22(19) 8 .
Sr4B Sr4B As3 52.15(12) 8 8
Zn2 Sr4B Sr1 63.8(3) . 8
Zn2 Sr4B Sr3 173.0(3) . 4_554
Zn2 Sr4B Sr4A 107.9(3) . 8
Zn2 Sr4B Sr4B 93.3(3) . 8
Zn2 Sr4B Sr4B 130.8(3) . 5
Zn2 Sr4B As1 107.5(3) . 20_656
Zn2 Sr4B As2 40.8(3) . .
Zn2 Sr4B As3 121.5(3) . 5
Zn2 Sr4B As3 47.8(3) . 8
Zn2 Sr4B As3 114.6(3) . .
As1 Sr4B Sr1 145.51(17) 20_656 8
As1 Sr4B Sr3 70.22(12) 20_656 4_554
As1 Sr4B Sr4A 56.39(9) 20_656 8
As1 Sr4B Sr4B 121.12(11) 20_656 5
As1 Sr4B Sr4B 54.37(10) 20_656 8
As1 Sr4B As2 142.3(2) 20_656 .
As1 Sr4B As3 107.79(17) 20_656 .
As1 Sr4B As3 95.70(13) 20_656 8
As2 Sr4B Sr4A 138.41(15) . 8
As2 Sr4B Sr4B 94.81(9) . 5
As3 Sr4B Sr1 55.88(9) . 8
As3 Sr4B Sr1 108.42(15) 5 8
As3 Sr4B Sr1 52.73(7) 8 8
As3 Sr4B Sr3 65.42(12) 5 4_554
As3 Sr4B Sr4A 63.54(9) 8 8
As3 Sr4B Sr4A 130.54(19) 5 8
As3 Sr4B Sr4A 56.20(9) . 8
As3 Sr4B Sr4B 67.05(14) . 8
As3 Sr4B Sr4B 54.79(13) 5 5
As3 Sr4B Sr4B 116.1(2) 8 5
As3 Sr4B Sr4B 144.6(3) 5 8
As3 Sr4B Sr4B 45.77(13) . 5
As3 Sr4B As1 104.21(16) 5 20_656
As3 Sr4B As2 86.50(13) 5 .
As3 Sr4B As2 105.63(14) . .
As3 Sr4B As2 76.12(10) 8 .
As3 Sr4B As3 75.60(12) . 8
As3 Sr4B As3 159.95(18) 5 8
As3 Sr4B As3 100.09(17) 5 .
Sr2A Zn1 Sr2A 130.05(3) 29 15_444
Sr2A Zn1 Sr2A 130.05(3) 8 29
Sr2A Zn1 Sr2A 73.33(5) 8 15_444
Sr2A Zn1 Sr2A 73.33(5) 22_556 29
Sr2A Zn1 Sr2A 130.05(3) 8 22_556
Sr2A Zn1 Sr2A 130.05(3) 22_556 15_444
Zn2 Zn1 Sr2A 83.0(3) 12_454 8
Zn2 Zn1 Sr2A 115.7(2) 12_454 29
Zn2 Zn1 Sr2A 115.7(2) 18_556 15_444
Zn2 Zn1 Sr2A 110.0(3) 3_545 8
Zn2 Zn1 Sr2A 49.2(3) 3_545 29
Zn2 Zn1 Sr2A 110.0(3) 12_454 15_444
Zn2 Zn1 Sr2A 49.2(3) 12_454 22_556
Zn2 Zn1 Sr2A 110.0(3) 18_556 22_556
Zn2 Zn1 Sr2A 49.2(3) 25 15_444
Zn2 Zn1 Sr2A 83.0(3) 25 22_556
Zn2 Zn1 Sr2A 83.0(3) 3_545 15_444
Zn2 Zn1 Sr2A 83.0(3) 18_556 29
Zn2 Zn1 Sr2A 49.2(3) 18_556 8
Zn2 Zn1 Sr2A 110.0(3) 25 29
Zn2 Zn1 Sr2A 115.7(2) 3_545 22_556
Zn2 Zn1 Sr2A 115.7(2) 25 8
Zn2 Zn1 Zn2 91.07(7) 18_556 3_545
Zn2 Zn1 Zn2 164.3(5) 18_556 25
Zn2 Zn1 Zn2 91.07(7) 25 12_454
Zn2 Zn1 Zn2 91.07(7) 25 3_545
Zn2 Zn1 Zn2 164.3(5) 12_454 3_545
Zn2 Zn1 Zn2 91.07(7) 18_556 12_454
As2 Zn1 Sr2A 57.24(3) 25 29
As2 Zn1 Sr2A 57.24(3) 3_545 8
As2 Zn1 Sr2A 87.16(3) 25 15_444
As2 Zn1 Sr2A 158.21(3) 25 8
As2 Zn1 Sr2A 87.16(3) 3_545 29
As2 Zn1 Sr2A 158.21(3) 18_556 15_444
As2 Zn1 Sr2A 70.26(3) 18_556 29
As2 Zn1 Sr2A 87.16(3) 18_556 8
As2 Zn1 Sr2A 70.26(3) 3_545 15_444
As2 Zn1 Sr2A 158.21(3) 3_545 22_556
As2 Zn1 Sr2A 57.24(3) 12_454 15_444
As2 Zn1 Sr2A 70.26(3) 25 22_556
As2 Zn1 Sr2A 70.26(3) 12_454 8
As2 Zn1 Sr2A 87.16(3) 12_454 22_556
As2 Zn1 Sr2A 57.24(3) 18_556 22_556
As2 Zn1 Sr2A 158.21(3) 12_454 29
As2 Zn1 Zn2 52.8(3) 25 25
As2 Zn1 Zn2 113.5(3) 25 12_454
As2 Zn1 Zn2 52.8(3) 18_556 18_556
As2 Zn1 Zn2 139.0(3) 18_556 25
As2 Zn1 Zn2 56.7(3) 18_556 12_454
As2 Zn1 Zn2 139.0(3) 25 18_556
As2 Zn1 Zn2 113.5(3) 3_545 25
As2 Zn1 Zn2 113.5(3) 12_454 18_556
As2 Zn1 Zn2 52.8(3) 12_454 12_454
As2 Zn1 Zn2 113.5(3) 18_556 3_545
As2 Zn1 Zn2 56.7(3) 3_545 18_556
As2 Zn1 Zn2 139.0(3) 12_454 3_545
As2 Zn1 Zn2 52.8(3) 3_545 3_545
As2 Zn1 Zn2 56.7(3) 25 3_545
As2 Zn1 Zn2 139.0(3) 3_545 12_454
As2 Zn1 Zn2 56.7(3) 12_454 25
As2 Zn1 As2 107.466(18) 12_454 18_556
As2 Zn1 As2 113.56(4) 25 18_556
As2 Zn1 As2 107.466(18) 25 12_454
As2 Zn1 As2 107.466(18) 3_545 25
As2 Zn1 As2 113.56(4) 3_545 12_454
As2 Zn1 As2 107.466(18) 3_545 18_556
Sr1 Zn2 Sr3 114.6(4) 8 .
Sr2A Zn2 Sr1 110.3(4) 23_666 8
Sr2A Zn2 Sr2B 2.5(3) 23_666 23_666
Sr2A Zn2 Sr3 72.5(3) 23_666 .
Sr2A Zn2 Sr4B 151.6(5) 23_666 .
Sr2A Zn2 Zn1 80.1(4) 23_666 25
Sr2B Zn2 Sr1 112.1(5) 23_666 8
Sr2B Zn2 Sr3 73.5(3) 23_666 .
Sr4A Zn2 Sr1 80.7(4) . 8
Sr4A Zn2 Sr2A 151.2(6) . 23_666
Sr4A Zn2 Sr2B 152.1(7) . 23_666
Sr4A Zn2 Sr3 78.7(4) . .
Sr4A Zn2 Sr4B 10.0(2) . .
Sr4A Zn2 Zn1 117.2(6) . 25
Sr4A Zn2 As2 97.4(6) . 20_656
Sr4A Zn2 As2 94.4(5) . .
Sr4A Zn2 As3 90.7(5) . 8
Sr4B Zn2 Sr1 71.0(3) . 8
Sr4B Zn2 Sr2B 153.3(5) . 23_666
Sr4B Zn2 Sr3 81.2(3) . .
Sr4B Zn2 Zn1 124.1(5) . 25
Zn1 Zn2 Sr1 123.0(4) 25 8
Zn1 Zn2 Sr2B 77.7(4) 25 23_666
Zn1 Zn2 Sr3 121.7(4) 25 .
As2 Zn2 Sr1 177.5(5) 20_656 8
As2 Zn2 Sr1 63.9(3) . 8
As2 Zn2 Sr2A 114.4(5) . 23_666
As2 Zn2 Sr2A 70.6(3) 20_656 23_666
As2 Zn2 Sr2B 68.8(4) 20_656 23_666
As2 Zn2 Sr2B 113.5(5) . 23_666
As2 Zn2 Sr3 63.2(3) 20_656 .
As2 Zn2 Sr3 173.1(5) . .
As2 Zn2 Sr4B 107.0(5) 20_656 .
As2 Zn2 Sr4B 92.0(4) . .
As2 Zn2 Zn1 61.2(3) . 25
As2 Zn2 Zn1 59.4(3) 20_656 25
As2 Zn2 As2 118.1(5) . 20_656
As2 Zn2 As3 116.6(4) 20_656 8
As2 Zn2 As3 123.8(5) . 8
As3 Zn2 Sr1 61.9(3) 8 8
As3 Zn2 Sr2A 73.0(3) 8 23_666
As3 Zn2 Sr2B 75.4(4) 8 23_666
As3 Zn2 Sr3 57.2(2) 8 .
As3 Zn2 Sr4B 84.0(4) 8 .
As3 Zn2 Zn1 151.9(5) 8 25
Sr1 As1 Sr1 122.61(5) 8 10_454
Sr1 As1 Sr2A 76.88(4) 8 15_444
Sr1 As1 Sr2A 80.07(4) 8 .
Sr1 As1 Sr2A 76.88(4) 10_454 .
Sr1 As1 Sr2A 80.07(4) 10_454 15_444
Sr1 As1 Sr3 140.643(18) 8 25
Sr1 As1 Sr3 70.11(3) 10_454 25
Sr1 As1 Sr4A 85.64(2) 8 27_565
Sr1 As1 Sr4A 143.32(3) 10_454 27_565
Sr1 As1 Sr4A 143.32(3) 8 30
Sr1 As1 Sr4A 85.64(2) 10_454 30
Sr2A As1 Sr2A 130.84(7) . 15_444
Sr2A As1 Sr3 137.58(4) . 25
Sr2A As1 Sr3 68.71(2) 15_444 25
Sr2B As1 Sr1 79.6(2) 15_444 10_454
Sr2B As1 Sr1 72.1(2) . 10_454
Sr2B As1 Sr1 79.6(2) . 8
Sr2B As1 Sr1 72.1(2) 15_444 8
Sr2B As1 Sr2A 124.90(17) . 15_444
Sr2B As1 Sr2A 6.38(17) 15_444 15_444
Sr2B As1 Sr2A 124.90(17) 15_444 .
Sr2B As1 Sr2A 6.38(17) . .
Sr2B As1 Sr2B 119.1(4) . 15_444
Sr2B As1 Sr3 74.64(17) 15_444 25
Sr2B As1 Sr3 136.2(2) . 25
Sr2B As1 Sr4A 141.41(18) . 27_565
Sr2B As1 Sr4A 141.41(18) 15_444 30
Sr2B As1 Sr4A 89.1(2) . 30
Sr2B As1 Sr4A 89.1(2) 15_444 27_565
Sr4A As1 Sr2A 85.16(3) 30 .
Sr4A As1 Sr2A 135.52(3) 27_565 .
Sr4A As1 Sr2A 135.52(3) 30 15_444
Sr4A As1 Sr2A 85.16(3) 27_565 15_444
Sr4A As1 Sr3 66.81(3) 30 25
Sr4A As1 Sr3 73.26(4) 27_565 25
Sr4A As1 Sr4A 81.76(5) 27_565 30
Sr4B As1 Sr1 101.76(12) 27_565 8
Sr4B As1 Sr1 125.21(11) 27_565 10_454
Sr4B As1 Sr1 125.21(11) 30 8
Sr4B As1 Sr1 101.76(12) 30 10_454
Sr4B As1 Sr2A 146.90(11) 27_565 .
Sr4B As1 Sr2A 80.71(10) 27_565 15_444
Sr4B As1 Sr2A 80.71(10) 30 .
Sr4B As1 Sr2A 146.90(11) 30 15_444
Sr4B As1 Sr2B 153.3(2) 27_565 .
Sr4B As1 Sr2B 86.0(2) 30 .
Sr4B As1 Sr2B 86.0(2) 27_565 15_444
Sr4B As1 Sr2B 153.3(2) 30 15_444
Sr4B As1 Sr3 55.10(11) 27_565 25
Sr4B As1 Sr3 80.74(10) 30 25
Sr4B As1 Sr4A 73.77(11) 30 27_565
Sr4B As1 Sr4A 18.26(11) 27_565 27_565
Sr4B As1 Sr4A 73.77(11) 27_565 30
Sr4B As1 Sr4A 18.26(11) 30 30
Sr4B As1 Sr4B 71.3(2) 27_565 30
As4 As1 Sr1 61.31(3) . 8
As4 As1 Sr1 61.31(3) . 10_454
As4 As1 Sr2A 65.42(3) . .
As4 As1 Sr2A 65.42(3) . 15_444
As4 As1 Sr2B 59.55(18) . 15_444
As4 As1 Sr2B 59.55(18) . .
As4 As1 Sr3 116.80(3) . 25
As4 As1 Sr4A 139.12(2) . 30
As4 As1 Sr4A 139.12(2) . 27_565
As4 As1 Sr4B 144.37(10) . 27_565
As4 As1 Sr4B 144.37(10) . 30
Sr1 As2 Sr1 81.42(3) 8 4_554
Sr1 As2 Sr2A 70.28(3) 4_554 14_554
Sr1 As2 Sr2A 126.82(4) 8 14_554
Sr1 As2 Sr2B 64.86(16) 4_554 14_554
Sr1 As2 Sr2B 144.3(2) 8 5
Sr1 As2 Sr2B 126.0(2) 8 14_554
Sr1 As2 Sr3 70.94(3) 8 27_565
Sr1 As2 Sr3 70.67(3) 4_554 27_565
Sr1 As2 Sr4A 137.12(4) 4_554 27_565
Sr1 As2 Sr4A 83.47(3) 8 27_565
Sr2A As2 Sr1 142.83(5) 5 8
Sr2A As2 Sr1 82.54(4) 5 4_554
Sr2A As2 Sr2A 77.54(5) 5 14_554
Sr2A As2 Sr2B 6.25(19) 5 5
Sr2A As2 Sr2B 75.1(2) 5 14_554
Sr2A As2 Sr3 72.15(4) 5 27_565
Sr2A As2 Sr4A 85.90(4) 5 27_565
Sr2A As2 Sr4A 143.56(5) 5 .
Sr2B As2 Sr1 78.0(2) 5 4_554
Sr2B As2 Sr2A 5.84(15) 14_554 14_554
Sr2B As2 Sr2A 72.08(19) 5 14_554
Sr2B As2 Sr2B 69.4(3) 5 14_554
Sr2B As2 Sr3 74.8(2) 5 27_565
Sr2B As2 Sr4A 92.15(18) 5 27_565
Sr3 As2 Sr2A 132.84(3) 27_565 14_554
Sr3 As2 Sr2B 127.17(16) 27_565 14_554
Sr3 As2 Sr4A 66.48(3) 27_565 27_565
Sr4A As2 Sr1 69.42(3) . 8
Sr4A As2 Sr1 89.37(3) . 4_554
Sr4A As2 Sr2A 66.31(4) . 14_554
Sr4A As2 Sr2A 145.91(4) 27_565 14_554
Sr4A As2 Sr2B 138.37(19) . 5
Sr4A As2 Sr2B 149.19(19) 27_565 14_554
Sr4A As2 Sr2B 69.3(2) . 14_554
Sr4A As2 Sr3 137.72(4) . 27_565
Sr4A As2 Sr4A 121.92(3) . 27_565
Zn1 As2 Sr1 136.71(3) 25 8
Zn1 As2 Sr1 134.42(4) 25 4_554
Zn1 As2 Sr2A 75.80(4) 25 5
Zn1 As2 Sr2A 66.15(3) 25 14_554
Zn1 As2 Sr2B 76.6(2) 25 5
Zn1 As2 Sr2B 70.96(17) 25 14_554
Zn1 As2 Sr3 135.30(4) 25 27_565
Zn1 As2 Sr4A 85.24(3) 25 .
Zn1 As2 Sr4A 81.07(3) 25 27_565
Zn2 As2 Sr1 73.6(3) . 8
Zn2 As2 Sr1 123.7(3) . 4_554
Zn2 As2 Sr1 114.6(3) 27_565 8
Zn2 As2 Sr1 131.6(3) 27_565 4_554
Zn2 As2 Sr2A 56.6(3) 27_565 5
Zn2 As2 Sr2A 117.9(3) 27_565 14_554
Zn2 As2 Sr2A 141.8(3) . 5
Zn2 As2 Sr2A 85.9(3) . 14_554
Zn2 As2 Sr2B 90.9(4) . 14_554
Zn2 As2 Sr2B 142.0(4) . 5
Zn2 As2 Sr2B 119.4(4) 27_565 14_554
Zn2 As2 Sr2B 62.7(3) 27_565 5
Zn2 As2 Sr3 72.6(3) 27_565 27_565
Zn2 As2 Sr3 138.7(3) . 27_565
Zn2 As2 Sr4A 89.3(3) . 27_565
Zn2 As2 Sr4A 32.1(3) 27_565 27_565
Zn2 As2 Sr4A 34.8(3) . .
Zn2 As2 Sr4A 138.8(3) 27_565 .
Zn2 As2 Zn1 63.9(3) 27_565 25
Zn2 As2 Zn1 66.1(3) . 25
Zn2 As2 Zn2 104.7(3) . 27_565
Sr1 As3 Sr1 71.81(3) 8 .
Sr1 As3 Sr2A 77.01(4) 8 10_454
Sr1 As3 Sr2A 103.86(5) . 26_545
Sr1 As3 Sr2A 158.81(5) 8 26_545
Sr1 As3 Sr2B 106.1(2) . 26_545
Sr1 As3 Sr2B 156.9(2) 8 26_545
Sr1 As3 Sr4A 87.68(3) 8 5
Sr1 As3 Sr4A 145.15(4) . 5
Sr1 As3 Sr4A 111.36(4) 8 8
Sr1 As3 Sr4A 67.80(3) . 8
Sr2A As3 Sr1 77.71(4) 10_454 .
Sr2A As3 Sr2A 81.80(5) 10_454 26_545
Sr2A As3 Sr2B 80.04(19) 10_454 26_545
Sr2A As3 Sr2B 3.3(2) 26_545 26_545
Sr2A As3 Sr4A 84.78(4) 26_545 8
Sr2A As3 Sr4A 70.25(4) 10_454 5
Sr2A As3 Sr4A 85.09(4) 26_545 5
Sr2A As3 Sr4A 138.56(5) 10_454 8
Sr2B As3 Sr1 73.1(2) 10_454 .
Sr2B As3 Sr1 71.5(2) 10_454 8
Sr2B As3 Sr2A 87.38(19) 10_454 26_545
Sr2B As3 Sr2A 6.46(19) 10_454 10_454
Sr2B As3 Sr2B 85.8(3) 10_454 26_545
Sr2B As3 Sr3 146.1(2) 10_454 4_554
Sr2B As3 Sr4A 136.8(2) 10_454 8
Sr2B As3 Sr4A 73.8(2) 10_454 5
Sr2B As3 Sr4B 139.6(2) 10_454 .
Sr3 As3 Sr1 124.12(4) 4_554 8
Sr3 As3 Sr1 137.99(4) 4_554 .
Sr3 As3 Sr2A 73.39(4) 4_554 26_545
Sr3 As3 Sr2A 140.10(4) 4_554 10_454
Sr3 As3 Sr2B 73.4(2) 4_554 26_545
Sr3 As3 Sr4A 70.22(3) 4_554 8
Sr3 As3 Sr4A 76.84(3) 4_554 5
Sr3 As3 Sr4B 57.23(10) 4_554 .
Sr4A As3 Sr2B 87.9(2) 8 26_545
Sr4A As3 Sr2B 81.8(2) 5 26_545
Sr4A As3 Sr4A 147.05(4) 8 5
Sr4B As3 Sr1 160.43(12) 5 .
Sr4B As3 Sr1 106.48(10) . .
Sr4B As3 Sr1 93.53(11) 5 8
Sr4B As3 Sr1 70.30(10) . 8
Sr4B As3 Sr2A 85.05(12) 5 26_545
Sr4B As3 Sr2A 143.32(10) . 10_454
Sr4B As3 Sr2A 86.54(13) 5 10_454
Sr4B As3 Sr2A 129.75(11) . 26_545
Sr4B As3 Sr2B 130.3(2) . 26_545
Sr4B As3 Sr2B 82.2(2) 5 26_545
Sr4B As3 Sr2B 90.2(3) 5 10_454
Sr4B As3 Sr3 61.03(12) 5 4_554
Sr4B As3 Sr4A 71.23(10) . 8
Sr4B As3 Sr4A 91.88(10) . 5
Sr4B As3 Sr4A 16.44(12) 5 5
Sr4B As3 Sr4A 131.10(12) 5 8
Sr4B As3 Sr4B 79.44(17) 5 .
Zn2 As3 Sr1 70.5(3) 8 .
Zn2 As3 Sr1 136.9(3) 8 8
Zn2 As3 Sr2A 53.8(3) 8 26_545
Zn2 As3 Sr2A 113.8(3) 8 10_454
Zn2 As3 Sr2B 57.1(3) 8 26_545
Zn2 As3 Sr2B 115.4(4) 8 10_454
Zn2 As3 Sr3 75.4(3) 8 4_554
Zn2 As3 Sr4A 135.4(3) 8 5
Zn2 As3 Sr4A 33.2(3) 8 8
Zn2 As3 Sr4B 101.5(3) 8 .
Zn2 As3 Sr4B 127.5(3) 8 5
Sr1 As4 Sr1 140.79(3) 10_454 .
Sr1 As4 Sr1 70.88(3) 10_454 15_444
Sr1 As4 Sr1 70.88(3) 8 .
Sr1 As4 Sr1 140.79(3) 8 15_444
Sr1 As4 Sr1 133.23(8) 10_454 8
Sr1 As4 Sr1 111.40(7) . 15_444
Sr1 As4 Sr2A 78.66(4) 10_454 .
Sr1 As4 Sr2A 81.97(4) 8 .
Sr1 As4 Sr2A 78.66(4) 8 15_444
Sr1 As4 Sr2A 81.97(4) 10_454 15_444
Sr1 As4 Sr2B 142.1(2) 10_454 10_454
Sr1 As4 Sr2B 70.1(2) 10_454 8
Sr1 As4 Sr2B 70.1(2) 8 10_454
Sr1 As4 Sr2B 142.1(2) 8 8
Sr2A As4 Sr1 140.44(4) 15_444 15_444
Sr2A As4 Sr1 72.94(3) 15_444 .
Sr2A As4 Sr1 140.44(4) . .
Sr2A As4 Sr1 72.94(3) . 15_444
Sr2A As4 Sr2A 129.85(9) . 15_444
Sr2A As4 Sr2B 76.1(2) 15_444 8
Sr2A As4 Sr2B 135.93(19) . 8
Sr2A As4 Sr2B 135.93(19) 15_444 10_454
Sr2A As4 Sr2B 76.1(2) . 10_454
Sr2B As4 Sr1 74.9(2) 10_454 15_444
Sr2B As4 Sr1 69.8(2) . 15_444
Sr2B As4 Sr1 76.9(2) 15_444 8
Sr2B As4 Sr1 141.9(2) . .
Sr2B As4 Sr1 141.9(2) 15_444 15_444
Sr2B As4 Sr1 68.0(2) 10_454 .
Sr2B As4 Sr1 85.1(2) . 8
Sr2B As4 Sr1 74.9(2) 8 .
Sr2B As4 Sr1 68.0(2) 8 15_444
Sr2B As4 Sr1 76.9(2) . 10_454
Sr2B As4 Sr1 85.1(2) 15_444 10_454
Sr2B As4 Sr1 69.8(2) 15_444 .
Sr2B As4 Sr2A 131.8(2) 15_444 .
Sr2B As4 Sr2A 3.3(3) . .
Sr2B As4 Sr2A 131.8(2) . 15_444
Sr2B As4 Sr2A 3.3(3) 15_444 15_444
Sr2B As4 Sr2B 76.3(5) 15_444 8
Sr2B As4 Sr2B 133.9(5) . 15_444
Sr2B As4 Sr2B 132.7(4) 15_444 10_454
Sr2B As4 Sr2B 111.3(5) 10_454 8
Sr2B As4 Sr2B 76.3(5) . 10_454
Sr2B As4 Sr2B 132.7(4) . 8
As1 As4 Sr1 124.30(3) . .
As1 As4 Sr1 66.62(4) . 10_454
As1 As4 Sr1 124.30(3) . 15_444
As1 As4 Sr1 66.62(4) . 8
As1 As4 Sr2A 64.93(5) . .
As1 As4 Sr2A 64.93(5) . 15_444
As1 As4 Sr2B 67.0(2) . 15_444
As1 As4 Sr2B 67.0(2) . .
As1 As4 Sr2B 124.4(2) . 8
As1 As4 Sr2B 124.4(2) . 10_454
As4 As4 Sr1 55.70(3) 10_454 .
As4 As4 Sr1 113.38(4) 10_454 10_454
As4 As4 Sr1 113.38(4) 10_454 8
As4 As4 Sr1 55.70(3) 10_454 15_444
As4 As4 Sr2A 115.07(5) 10_454 .
As4 As4 Sr2A 115.07(5) 10_454 15_444
As4 As4 Sr2B 113.0(2) 10_454 .
As4 As4 Sr2B 55.6(2) 10_454 10_454
As4 As4 Sr2B 55.6(2) 10_454 8
As4 As4 Sr2B 113.0(2) 10_454 15_444
As4 As4 As1 180.0(4) 10_454 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sr1 Sr2B 3.733(11) 10_454
Sr1 Sr2B 3.643(10) 15_444
Sr1 Sr4A 3.6005(14) 8
Sr1 Sr4B 3.616(5) 8
Sr1 Zn2 3.432(13) 8
Sr1 As1 3.1950(11) 10_454
Sr1 As2 3.2132(13) 8
Sr1 As2 3.2354(12) 3_545
Sr1 As3 3.1797(13) 8
Sr1 As3 3.2115(13) .
Sr1 As4 3.0535(13) 10_454
Sr1 As4 3.3926(15) .
Sr2A Sr3 3.7576(17) 27_565
Sr2A Sr4A 3.712(2) 14_454
Sr2A Zn1 3.5281(18) 29_554
Sr2A Zn2 2.710(12) 31_565
Sr2A As1 3.2632(19) .
Sr2A As2 3.631(2) 14_454
Sr2A As2 3.060(2) 5
Sr2A As3 3.2121(18) 26
Sr2A As3 3.189(2) 10_454
Sr2A As4 3.6286(18) 10_454
Sr2A As4 3.2762(17) .
Sr2B Sr4A 3.797(13) 14_454
Sr2B Zn1 3.670(12) 29_554
Sr2B Zn2 3.065(16) 31_565
Sr2B As1 3.144(13) .
Sr2B As2 3.541(13) 14_454
Sr2B As2 3.217(12) 5
Sr2B As3 3.533(10) 26
Sr2B As3 3.056(12) 10_454
Sr2B As4 2.945(10) .
Sr2B As4 3.283(10) 10_454
Sr3 Sr4A 3.6361(10) 6
Sr3 Sr4A 3.6361(10) .
Sr3 Sr4B 2.957(6) 3_545
Sr3 Sr4B 2.957(6) 8
Sr3 Zn2 3.540(12) 6
Sr3 Zn2 3.540(12) .
Sr3 As1 3.3927(7) 20_656
Sr3 As1 3.3927(7) 25
Sr3 As2 3.3121(13) 23_666
Sr3 As2 3.3121(13) 20_656
Sr3 As3 3.0738(14) 3_545
Sr3 As3 3.0738(14) 8
Sr4A Sr4B 1.009(6) .
Sr4A Sr4B 3.696(5) 8
Sr4A Zn2 1.778(13) .
Sr4A As1 3.2057(14) 20_656
Sr4A As2 3.1079(13) .
Sr4A As2 3.3211(14) 20_656
Sr4A As3 3.2438(14) 8
Sr4A As3 3.2612(14) 5
Sr4B Sr4B 3.427(10) 8
Sr4B Sr4B 3.730(11) 5
Sr4B Zn2 2.712(14) .
Sr4B As1 2.941(5) 20_656
Sr4B As2 3.696(5) .
Sr4B As3 3.615(5) 8
Sr4B As3 3.100(6) .
Sr4B As3 2.719(5) 5
Zn1 Zn2 2.775(13) 25
Zn1 Zn2 2.775(13) 3_545
Zn1 Zn2 2.775(13) 12_454
Zn1 Zn2 2.775(13) 18_556
Zn1 As2 2.6597(9) 3_545
Zn1 As2 2.6597(9) 18_556
Zn1 As2 2.6597(9) 25
Zn1 As2 2.6597(9) 12_454
Zn2 As2 2.584(13) 20_656
Zn2 As2 2.417(12) .
Zn2 As3 2.691(13) 8
As1 As4 2.746(3) .
As4 As4 0.700(4) 10_454
